study on the shear strength of foundry sand cores using clay
A. I. OPALUWA
STUDY ON THE SHEAR STRENGTH OF FOUNDRY SAND
CORES USING CLAY AND CASSAVA STARCH AS BINDER
DEPT. OF METALLURGICAL & MATERIALS ENGINEERING, FEDERAL UNIVERSITY OF TECHNOLOGY, AKURE, NIGERIA
DEPT. OF FOUNDRY ENGINEERING, FEDERAL POLYTECHNIC, IDAH, NIGERIA
ABSTRACT: Sand cores for casting of intricate shapes were produced from Ojolofe silica sand using
cassava starch and Iyoloko clay, Idah Kogi State Nigeria as binders. Various compositions (6 – 12% water
4 – 12% cassava starch and 5% Iyoloko clay) with addition of Iyolofe silica sand were mixed together to
produce large number of standard cores samples of two different types (green and baked).
the cores samples were done at different temperatures ranging from 90 and 200oC for 60 – 150
minutes. Thereafter, determination of green and baked shear strengths was carried out on a large
number of green and baked cores samples using universal tensile machine through standard
procedure. It was found that appropriate baking conditions and optimum core mixtures were
established for cassava starch/clay bonded cores; and clay addition was found to increase both the
green and baked strengths values. The optimum clay/starch core mixture with the best shear strength
values was found to be core with
10% starch, 10% water and 5% clay; the appropriate baking
temperature and time 2were 180oC and 22 hours respectively. Their green and baked shear strength
values were 31.1 KN/m and 498.1 KN/m respectively. These values were found to be adequate for
production of strong sand cores using starch/cay as binders for non - ferrous and ferrous castings as
collaborated by successfully casting of a T – joint pipe aluminum casting. Finally, the research showed
that good cores can be produced using cassava starch/clay as binders as rationale behind the work.
KEYWORDS: Cassava Starch, Cores, Binders, Shear Strength, Clay and Foundry sand
There are several foundry industries in Nigeria that sourced raw materials (silica sand, clay,
binders and additives) used for producing effective foundry sand cores from overseas in 70s so there is
need to develop appropriate molding raw materials since all foundry works depended exclusively on
imported raw materials including even the molding sand (Ihom et al, 2006). In sand casting operations,
sand is used as a molding material to form the external shape of the cast component or as a core
material to create internal cavities in castings such as engine blocks (Abdulwahab et al., 2008).
There is a great need to be familiar with the utilization, design and production of suitable cores
because cores are crucial to achieving efficient production of cast products with hollow cavities. In
fact there are no ways of doing this without the use of cores if excessive foundry wastes and machine
scraps were to be eliminated (Charles, 2004).
Sand grains cannot adhere to each other without the introduction of binders that cause them to
stick together and produce the cavity into which molten metal is introduced (Brown, 1994). Oyetunji
and Seidu (2012) studied the synergistic effects of starch and rubber-latex as core binders for foundry
sand cores production. Clay is the general-purpose binder for sand castings and a lot of work has been
done in the area of developing suitable clays for sand moulds. Binders are introduced into the
moulding and core mixtures in order to improve their properties especially the strength (Nwajagu,
1994). While clay has been found to be satisfactorily used as a binder for molding sands, it is largely
unsatisfactory when used singly as a binder for core production. Some of the common binders for core
making are vegetable oil, honey, Soya beans, cotton seed, ground nut, palm kernel, beniseed, cashew
nut and castor oils (Colin, 2008). The use of cassava starch for sand core production has not been
extensively reported in the literature, and hence the need to investigate its potential in this respect.
Since cassava is a cheap source of abundant starch with excellent bonding characteristics, cassava
starch has therefore been chosen for the investigation.
This work is aimed at producing sand cores using cassava starch and clay as binders and
evaluating their suitability for the casting of aluminum alloy T-Joint pipe while the objective of this
work are to utilize locally sourced raw materials (cassava starch, Iyoloko clay and Ojolofe sand) to
produce cores and determine their green and baked shear strengths property.
The work uses locally produced binders, cassava starch and clay, that constitute no health
hazards and are environmental friendly for the production of sand cores. In addition, the utilization
© copyright FACULTY of ENGINEERING ‐ HUNEDOARA, ROMANIA 155 ANNALS OF FACULTY ENGINEERING HUNEDOARA – International Journal Of Engineering of these binders will reduce the dependence on imported materials for the production of some cast
products. In doing this it will promote the development of indigenous technology needed for local
production of intricate machine parts such as engine block at reduced costs and for self-reliance.
Finally this work will promote economic growth of the country by generating internal revenue and
preserving foreign earnings for economic development.
The scope of this work entails production of cassava starch and clay bonded sand cores using
river Niger sand collected from Ojolofe water side in Idah local government area of Kogi State Nigeria
while the clay was from Iyoloko stream at Ede-Alaba also in Idah local government area in Kogi State
Nigeria. Production of different cores of various compositions (6% to 12% water, 4% to 12% cassava
starch and 5% clay) was carried out. Evaluations of green and baked shear strengths were carried out.
To be able to establish optimum baking condition and optimum core mixture, several cores mixtures
were produced at varying baking times and temperatures for its shear strength determination.
MATERIALS AND EQUIPMENT
Materials used for this work were silica sand collected from Ojolofe water side in Idah local
government area of Kogi State Nigeria, Iyoloko clay collected from Iyoloko stream at Ede-Alaba in Idah
local government area 0f Kogi state, cassava starch which was extracted from cassava tubers obtained
from Akure in Ondo state Nigeria and tap water was used for tempering.
Equipment used are weighing, mixer or muller, measuring cylinder, specimen rammer,
permeability meter, universal strength testing machine, oven, sieve shaker and sets of sieve, crucible
furnace, hack saw, mould box, core box, wire brush and chisel.
(i) Cassava Starch Preparation
Cassava tubers were peeled and properly washed. The washed tubers were pounded followed by
grinding into pulp. Water was then added to easy the extraction of starch. On the addition of water,
it formed suspension which was left to stay for 2 hours before the water above was decanted. The
starch residue was properly dried to white, odorless and tasteless powder in accordance with Anonim,
2009, Oyetunji and Seidu, 2012 and Narayana, 2002.
(ii) Sand preparation
The sand was collected from the site, washed to remove clay and other impurities. It was
properly dried and sieved using shaker on which meshes of different aperture were mounted. The clay
was collected from the site and pebbles were removed from it. After drying, both the clay and the
sand were sent for mineralogical composition analysis using ED X-ray Fluorescence Analyzer in
accordance with Ayoola, 2010. The results of the mineralogical composition are as shown in Table 1.
Table 1: Mineralogical Composition of Ojolofe Silica Sand and Iyoloko Clay
The sieve analysis was done to determine the grain size in accordance with Oyetunji and Omole,
2011; and Ayoola, 2010 and the result shown in Table 2.
Table 2: The Sieve Analysis of Ojolofe Silica Sand
Less or equal 63
Average Grain Size (micrometer) = Total Product
Total % sand retained
(iii) Selection of Core Mixture
For this work, a large number of cores from mixtures, based on the proportion of the
constituent of sand, cassava starch, clay and water, were prepared. The starch/clay bonded cores
156 Tome XI (Year 2013). Fascicule 3. ISSN 1584 – 2673 ANNALS OF FACULTY ENGINEERING HUNEDOARA – International Journal Of Engineering were produced from mixtures containing compositions (6-12% water, 4-12% starch 5% clay). The full
composition of core mixture is in Table 3
Table 3: Composition of the Core Mixtures used in the Investigations
Starch and Clay mixture
6% water + 4% starch
6% water + 6% starch
6% water + 8% starch + 5% clay
6% water + 10% starch
6% water + 12% starch
8% water + 4% starch
8% water + 6% starch
8% water + 8% starch + 5% clay
8% water + 10% starch
8% water + 12% starch
Starch and Clay mixture
10% water + 4% starch
10% water + 6% starch
10% water + 8% starch + 5% clay
10% water + 10% starch
10% water + 12% starch
12% water + 4% starch
12% water + 6% starch
12% water + 8% starch + 5% clay
12% water + 10% starch
12% water + 12% starch
(iv) Production of Test Specimens
After the mixtures were properly mixed and blended, 50 test samples of 50 mm diameter by 56
mm height were made from each of the mixtures. This was done by ramming the mixture in the
sleeves of 50 mm diameter and to a height of 56 mm. Ramming was accomplished by dropping a
rammer of 5Kg mass three times from a height of 50 mm. The core specimen was ejected from sleeve
by a piston.
(v) Core Baking Procedure
Core baking was carried out in an oven capable of attaining a temperature of 500oC and with
capacity for 40 cores at a time. Each batch of cores was introduced into the furnace on steel plates
after the requisite temperature had been attained and maintained for a predetermined period. The
oven had an extraction system for removing the moisture produced during baking. This arrangement
ensures a uniform and standard baking procedure (Giesseren, 2004).
The following tests were performed on the produced cores:
(a) Green Shear Strength Test
Determination of green shear strength values was carried out using the universal sand testing
machine. The specimen to be tested was mounted on a stripping post and a shear load was gradually
applied by turning a hand wheel until fracture. The fracture load was automatically recorded on the
attached scale (Jain, 2008, Fayomi, et al 2011, Ademoh, 2008 and Oyetunji et al., 2009).
(b) Baked Shear Strength Test
Based on the results from the green strength values, starch/clay cores of different compositions
were produced using 10% starch, 5% clay and 10% water. The cores were baked at various
temperatures between 90 and 180oC and for different baking periods between 1 and 21/2 hours. Baked
shear strength values were determined using the universal sand testing machine. The specimens were
tested for baked shear strength (Jain, 2008; Fayomi, et al 2011, Ademoh, 2008).
(c) Determination of Appropriate Baking Temperatures
For the appropriate baking temperature to be obtained, a large number of cores from a variety
of core mixtures at different water content were produced and baked at various temperatures of
between 90 and 200oC for a fixed time of two hours. The baked cores were later tested for shear
strength using the universal sand testing machine in accoradance with standard procedures Fayomi, et
DISCUSSION OF THE RESULTS - Mineralogical Analysis of the Sand
The Ojolofe sand and Iyoloko clay mineralogical analysis in Table 1, the Ojolofe sand contains
95.30% Si02 and 0.55% Al203. The silica content of 95.30% compares well with the minimum acceptable
values of 95% recommended for moulding and core sands (Brown, 2000). A high silica value is
necessary to withstand the heat of molten metal during casting and increase its refractioness (Jain,
2008). The Iyoloko clay, on the other hand, had 65.40% silica and 20.30% alumina as the principal
constituents. These values are common and adequate for general purpose foundry moulding sand and
cores. The higher alumina content provides the necessary refractoriness needed by cores (Brown,
Sand Grain Size
Table 2 shows the sieve analysis of Ojolofe sand used for the production of the core. The sand
has an average grain size of 184.03 micron meters which is within the AFS acceptable size range of
between 180 and 250 microns used in Foundry. It is clearly on the fine side for mould production but
specifically suitable for core making in providing the necessary green and baked strength values,
adequate flowability, and good mouldability and permeability (Ihom, et al 2006).
Green Shear Strength Values
In Figure 1, the green shear strengths increased with water content reaching a maximum value
at 10% irrespective of the starch level. The green strength values were generally high for cores
Tome XI (Year 2013). Fascicule 3. ISSN 1584 – 2673 157 ANNALS OF FACULTY ENGINEERING HUNEDOARA – International Journal Of Engineering containing 6 – 10% water and dropped sharply for all cores with 12% water content. This sharp drop
was because of excessive wetness resulting not only in low green shear values, but also difficulty on
moulding. The maximum green strength 31.1 KN/m2 was obtained for the starch/clay bonded cores
produced from a mixture containing 10% starch, 5% clay and 10% water. From the results of green
shear strength values in Figure 1, it is clear that starch/clay cores have adequate strength values. This
is in comparison with the minimum acceptable value of 10.0KNm-2 for organic-bonded cores. The
strongest cores were produced from core mixtures of 10% starch, 10% water and 5% clay compositions.
Green Shear Strength
4% Starch +
6% Starch +
8% Starch +
12% Starch +
Baked Shear Strength
Figure 1: Variation of Green Shear Strength with Water on Starch/Clay bonded Cores
Baked Shear Strength of Starch bonded Cores
Figure 2 shows the effect of baking temperature and baking time on the shear strengths for
clay-starch bonded cores produced from mixes of 10% starch, 10% water and 5% clay. These values
were based on the maximum strength values obtained from the preliminary investigation. It is seen in
Figure 2 that maximum baked shear strengths were obtained for cores when baking was carried out at
180oC for 2 hours. This means that optimum baked shear strength values will not be achieved when
these cores are baked outside this specification since polymerization will start. The maximum shear
strength for the starch/clay cores was 498.1 KNm-2. This baked strength value agrees very well with
standard value of between 400KNm-2 and 600KNm-2 needed for nonferrous and iron castings (Fayomi et
Baking Time (hr)
Figure 2: Variation of Baked Shear Strength with Baking Time for Clay-Starch Cores (10% Starch, 10%
Water and 5% clay)
Baked Shear Strength versus Baking Temperature for Starch-bonded Cores
Preliminary work was carried out to determine the optimum core mixture and appropriate
baking conditions for the starch/clay bonded cores. In this respect, baked shear strength values were
measured for cores produced from selected clay/starch additions at different water levels. For each
core mixture, baking temperature was varied between 90 and 200oC for two hours. The results are
contained in Figures 3–6. From the results, it is clear that clay additions into starch cores significantly
increased the baked shear strengths, which further increased as the starch/clay content increased.
For all the cores, there was an initial increase in the baked shear strength as the baking temperature
increased but attained maximum values at the baking temperature of 180oC for two hours for each
core mix. Form these figures; it was observed that good quality clay/starch cores can be produced
from core mixes containing 8-12% starch, 5% clay and 6-10% water after baking between 150 and 180oC
for 2 hours. For the mixes investigated, the strongest clay/starch cores were produced from mixes
containing 8 – 10 starch, 5% clay and 8 – 10% water.
158 Tome XI (Year 2013). Fascicule 3. ISSN 1584 – 2673 ANNALS OF FACULTY ENGINEERING HUNEDOARA – International Journal Of Engineering Figure 3: Variation of Baked Shear Strength with Baking Temperature
for Clay-Starch Cores with 6% Water
Figure 4: Variation of Baked Shear Strength with Baking Temperature for Clay-Starch
bonded Cores with 8% Water.
Figure 5: Variation of Baked Shear Strength with Baking Temperature
for Clay-Starch bonded Cores with 10% Water)
Figure 6: Variation of Baked Shear Strength with Baking Temperature for Clay-Starch bonded Cores
with 12% Water)
Tome XI (Year 2013). Fascicule 3. ISSN 1584 – 2673 159 ANNALS OF FACULTY ENGINEERING HUNEDOARA – International Journal Of Engineering Performance Evaluation Test
The cast aluminum T-joint pipes, which were produced using a clay/starch cores was found to be
of excellent quality and good finish. Satisfactory castings can certainly be produced using these core
mixtures containing 10% starch, 10% water and 5% clay.
The results obtained from the research has clearly shown that using the appropriate foundry
sand, good quality cores can be successfully produced using cassava starch in combination with Iyoloko
clay. Good quality cores can be produced from core mixtures containing 8-12% starch, 5% clay and 610% water after baking between 150 and 180oC for 2 hours. However, in this respect, cores with
optimum properties were from mixtures containing 10% starch, 5% clay and 10% water. The green and
baked shear strengths values from these tested cores were 31.1 KN/m2 and 498.1 KN/m2 respectively.
These green and baked shear strengths values obtained from these tested cores made them to be
suitable for applications in the production of iron and non-ferrous castings. The successful
performance evaluation test carried out in the casting of an aluminium T-joint pipe has proved this to
[1.] Abdulwahab, M, Gaminana, J.O, Bellow, K.A and Achuokpa, E.O (2008); Prospect of Local Core Binders in
Foundry Industries. Proceedings of Nigerian Metallurgical society. 25th Annual conference. Akure, 2008. Pp
Ademoh, N. A. (2009). Foundry Properties of sand cores bonded with compositions of Nigerian grades 1 and
2 acacia species with bentonite clay. International Journal of Physical Sciences Vol. 4 (5). Pp 330-335.
Ayoola, W.A; S. O. Adeosun, A. Oyetunji, and A.M. Olodoye (2010). Suitability of Oshogbo Sand Deposit as
Moulding Sand. The Kenya Journal of Mechanical Engineering (KJME). Vol.6 No.1. Pp. 33-41
Brown, J. R. (2000); Feseco Foundry Men’s Hand Book Feseco International Ltd, Birmingham. Pp 28-31.
Colin, C. (2006); Foundry oil Bonded Sand Core Production. Croucher of www.myhome foundry.com.
Charles, E. B. (2004). Advances in Core Making Technology. Penton media, Inc. Britain. P 2026.
Fayomi, O. S. I.; Ojo, O. I. and Popoola, A. P. I. (2011). Investigating (Ochadamu) silica sand, clay and local
oils for foundry core. International Journal of the Physical Sciences Vol. 6 (8) Pp. 1894-1904.
Giesseren, A. W. (2004). AWB-An Environment-friendly Core Production Technology. Documents and
settings/Inc18/my documents/AWB-an environment friendly core Production Technology of www.myhome
Foundry. Come. Pp 5-6.
Ihom, A.P, Jatau, J.S and Mohammed, M. H. (2006); Assessment of Honey as a Binder for Core Making in
Foundry. Proceeding of Nigeria Metallurgical Society. Abuja 2006. Pp 39-44.
Jain, P. L (2006); Principle of Foundry Technology. Tata, Mc Graw-Hill Publisher, New Delhi. Pp 55 – 120.
Jain, R.K (2008); Production Technology. Khanna Publishers, Nai Sarak, Delhi. India. Pp 138-244.
Oyetunji A; Bankole, L.K. and Alhassan, A.O. (2009). Binding Characteristics of Mbushi and Ewekoro Clays
of Nigeria in Foundry Moulding Sand. Global Journal of Engineering and Technology. (Volume 2, No. 4,
December 2009), Pp 509-514.
Oyetunji A. and Omole S.O. (2011) Evaluation of Ductile Iron Produced Using Rotary Furnace With
Variable Compositions Of Magnesium Addition. International Journal of Science and Advanced Technology
(ISSN 2221-8386) Volume 1 No 9 November 2011 http://www.ijsat.com Pp. 276 -282.
Oyetunji A. and Seidu, S. O. (2012). Synergistic Effects of Starch and Rubber-Latex As Core Binders For
Foundry Sand Cores Production. ACTA TECHNICA CORVINIENSIS. Bulletin of Engineering. Tome V. FASCICULE
4. Faculty of Engineering. University of Hunedoara, Romania. Pp.103-106. ISSN 2067-3807.
Narayana, S. (2002). Physicochemical and Functional Properties of Tropical Tuber Starches: A Review.
Nwajagu C. O (1994); Foundry Theory and Practice. ABC Publisher. Enugu.
ANNALS of Faculty Engineering Hunedoara
– International Journal of Engineering
copyright © UNIVERSITY POLITEHNICA TIMISOARA,
FACULTY OF ENGINEERING HUNEDOARA,
5, REVOLUTIEI, 331128, HUNEDOARA, ROMANIA
160 Tome XI (Year 2013). Fascicule 3. ISSN 1584 – 2673